﻿



Fig. 



l.-St 



ress-Strain Diagran 



. Specimen 



10. 





















J 



', 



^-.- 



X 



£Z 





§ 











9 



/, 



/ 



/I 









1 











/, 



/ 



/ 











1 









A 



/ 



/ 



/ 





<£ 5 







I 







^ 



'J 





^ 



/^ 



•J 













^y 



w 



u 



/V 



^J 





-i„ 









i 



J 



/ v 



7^ 



$ 



f^v 



// 



/ 











4 

 t i 



/ , 



/■ 



y 



' 



// 















/ 



/ 





/ 



y 



? 



Der 



'.: ■•■■■ 



ecTio 



! .'11 



















i 1 





,;;, * 



Ob 





m 



z \ 







Dec* 







71 



;:; ; 



Si :! 









OS 0107 OOf 

 05 OM CO? 

 ?.* °I70 °° 6 



Fig. 2.— Torsion-Stress-Strain Diagram. Specimen 1 D. 























^ 







* 











£ 



~$ 



t 



A 



7 



•* 





■e 













'- 



/, 



/ 



/ 







^ 











t 



/ 



/ 



A 









| 









2 



/ 



/ 



y 











v 







/ 



a 



/ 



Y 













<o 







M 





r. 





—SM. 











^ 





,/ 



c 



0/ 



# 















<C 





^ 



/, 



/ 



/ 













ooo 













OCFU 







,TU« 





» 



DO -ojoi -0 



000 -0 



02 



OS -0 



04 005 0O« 007 . £ 

 03 00* 005 006 



07 , 



08 



09 0." 



DECRUS. 



00 ob 





■' 



0, Jo 2 o'o3 00* " M 



00 ok,, -00, -003 00. C 



■m — £& m j°s «so n 



\ ; 



OS 007 



PMl.Mag.Ser.6,Vol.l2,Pl.X. 



Fig. 4.— Average Curves for Nickel-Steel. 

 Reversed immediately. 



Specimens A ; B ; C 



v. 



p- 



Fig. 5. — Average Curves in Torsion for Mild Carbon-Steel. 



































f^ 



i. 











1 























I 













^ 











I 









f^2- 





» r 5^ 











\ 









e"^ 



1^/ 













1 / 







/ 





















/ 



Qcfteci 



W/V P 



/? 7/7V7 



7-Z^/VC 



W ,„W 





00 .0 



00 :"? :° 



" :°o : :J 



" '0 



05 Z 



oi : 







s? -i 



+ .. 



7, * 



28 2 8S 3 



« 3 



ss -4 



50 S 



3 -t 



70 























, 







t 











<?z 















X 







V- 



^ 



/ 



s 

















0/ 



/ 



f .<* 

















1 





** 



ty 



^ 

















J 0. 



0/ 



, 



/ 























/ 



DiFltCT/OIYf 



CKVHt 



'i£HG 





W^J 





•0 





01 °° 





0? M -0 



il I 



11 I 



Ob -° 



00 3 



S| 00°8 



■0 



Debri 



£S. 



* , 



71 Z 



28 -, 



S3 , 



,2 -3 



SS •* 



50 -513 S 









Fig 



7.— Torsion 



Test of Coran 



on Wrought 



Iron. 



































































/ 























/.. 























/ 

















} 









/ 





// 











J 







/ 





// 













§ 





^ 



'/ 



*¥• 

















§ 









"¥ 

















>1 





L^/ 



/> 

















t 

























/ 



7 



7 





















/ 



/ 



/' 



^-f^t 







, ;OT! 



■urn 



!W. 





■0 





00 001 



of -0 



° : °o 



04 



11 ;°°| ;| 



Ss •( 



08 1 



0? 



■0 



Deant es 



28 -3 42 4 



56 -5 70 













Fig. 8.— Stress-Strain Diagram : Wrought Iron in torsion. 

 Specimens K. (Stay-bolt iron.) 



